LMucko/crystallography-open-database huggingface dataset:
Cation ordering in magnesioferrite, MgFe2O4, to 982 C using in situ synchrotron X-ray powder diffraction Sample: on cooling T = 715 C
Antao, S. M.; Hassan, I.; Parise, J. B.; American Mineralogist 90 (2005) 219–228; doi:10.2138/am.2005.1559

data_9003611
_publ_section_title
;
 Cation ordering in magnesioferrite, MgFe2O4, to 982 C using
 in situ synchrotron X-ray powder diffraction
 Sample: on cooling T = 715 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              219
_journal_page_last               228
_journal_paper_doi               10.2138/am.2005.1559
_journal_volume                  90
_journal_year                    2005
_chemical_formula_sum            'Fe2 Mg O4'
_chemical_name_mineral           Magnesioferrite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.45245
_cell_formula_units_Z            8
_cell_length_b                   8.45245
_cell_length_c                   8.45245
_cell_volume                     603.876
_database_code_amcsd             0003704
_diffrn_ambient_temperature      988.15
_exptl_crystal_density_diffrn    4.400
_exptl_crystal_thermal_history   'cooling T = 715 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Fe2 Mg) O4'
_cod_database_code               9003611
Cation ordering in magnesioferrite, MgFe2O4, to 982 C using in situ synchrotron X-ray powder diffraction Sample: on cooling T = 696 C
Antao, S. M.; Hassan, I.; Parise, J. B.; American Mineralogist 90 (2005) 219–228; doi:10.2138/am.2005.1559

data_9003612
_publ_section_title
;
 Cation ordering in magnesioferrite, MgFe2O4, to 982 C using
 in situ synchrotron X-ray powder diffraction
 Sample: on cooling T = 696 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              219
_journal_page_last               228
_journal_paper_doi               10.2138/am.2005.1559
_journal_volume                  90
_journal_year                    2005
_chemical_formula_sum            'Fe2 Mg O4'
_chemical_name_mineral           Magnesioferrite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.45180
_cell_formula_units_Z            8
_cell_length_b                   8.45180
_cell_length_c                   8.45180
_cell_volume                     603.737
_database_code_amcsd             0003705
_diffrn_ambient_temperature      969.15
_exptl_crystal_density_diffrn    4.401
_exptl_crystal_thermal_history   'cooling T = 696 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Fe2 Mg) O4'
_cod_database_code               9003612
Cation ordering in magnesioferrite, MgFe2O4, to 982 C using in situ synchrotron X-ray powder diffraction Sample: on cooling T = 658 C
Antao, S. M.; Hassan, I.; Parise, J. B.; American Mineralogist 90 (2005) 219–228; doi:10.2138/am.2005.1559

data_9003613
_publ_section_title
;
 Cation ordering in magnesioferrite, MgFe2O4, to 982 C using
 in situ synchrotron X-ray powder diffraction
 Sample: on cooling T = 658 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              219
_journal_page_last               228
_journal_paper_doi               10.2138/am.2005.1559
_journal_volume                  90
_journal_year                    2005
_chemical_formula_sum            'Fe2 Mg O4'
_chemical_name_mineral           Magnesioferrite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.44813
_cell_formula_units_Z            8
_cell_length_b                   8.44813
_cell_length_c                   8.44813
_cell_volume                     602.951
_database_code_amcsd             0003706
_diffrn_ambient_temperature      931.15
_exptl_crystal_density_diffrn    4.406
_exptl_crystal_thermal_history   'cooling T = 658 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Fe2 Mg) O4'
_cod_database_code               9003613
Cation ordering in magnesioferrite, MgFe2O4, to 982 C using in situ synchrotron X-ray powder diffraction Sample: on cooling T = 601 C
Antao, S. M.; Hassan, I.; Parise, J. B.; American Mineralogist 90 (2005) 219–228; doi:10.2138/am.2005.1559

data_9003614
_publ_section_title
;
 Cation ordering in magnesioferrite, MgFe2O4, to 982 C using
 in situ synchrotron X-ray powder diffraction
 Sample: on cooling T = 601 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              219
_journal_page_last               228
_journal_paper_doi               10.2138/am.2005.1559
_journal_volume                  90
_journal_year                    2005
_chemical_formula_sum            'Fe2 Mg O4'
_chemical_name_mineral           Magnesioferrite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.44122
_cell_formula_units_Z            8
_cell_length_b                   8.44122
_cell_length_c                   8.44122
_cell_volume                     601.472
_database_code_amcsd             0003707
_diffrn_ambient_temperature      874.15
_exptl_crystal_density_diffrn    4.417
_exptl_crystal_thermal_history   'cooling T = 601 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Fe2 Mg) O4'
_cod_database_code               9003614
Cation ordering in magnesioferrite, MgFe2O4, to 982 C using in situ synchrotron X-ray powder diffraction Sample: on cooling T = 562 C
Antao, S. M.; Hassan, I.; Parise, J. B.; American Mineralogist 90 (2005) 219–228; doi:10.2138/am.2005.1559

data_9003615
_publ_section_title
;
 Cation ordering in magnesioferrite, MgFe2O4, to 982 C using
 in situ synchrotron X-ray powder diffraction
 Sample: on cooling T = 562 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              219
_journal_page_last               228
_journal_paper_doi               10.2138/am.2005.1559
_journal_volume                  90
_journal_year                    2005
_chemical_formula_sum            'Fe2 Mg O4'
_chemical_name_mineral           Magnesioferrite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.43831
_cell_formula_units_Z            8
_cell_length_b                   8.43831
_cell_length_c                   8.43831
_cell_volume                     600.851
_database_code_amcsd             0003708
_diffrn_ambient_temperature      835.15
_exptl_crystal_density_diffrn    4.422
_exptl_crystal_thermal_history   'cooling T = 562 C'
_cod_original_cell_volume        600.850
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Fe2 Mg) O4'
_cod_database_code               9003615
Cation ordering in magnesioferrite, MgFe2O4, to 982 C using in situ synchrotron X-ray powder diffraction Sample: on cooling T = 543 C
Antao, S. M.; Hassan, I.; Parise, J. B.; American Mineralogist 90 (2005) 219–228; doi:10.2138/am.2005.1559

data_9003616
_publ_section_title
;
 Cation ordering in magnesioferrite, MgFe2O4, to 982 C using
 in situ synchrotron X-ray powder diffraction
 Sample: on cooling T = 543 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              219
_journal_page_last               228
_journal_paper_doi               10.2138/am.2005.1559
_journal_volume                  90
_journal_year                    2005
_chemical_formula_sum            'Fe2 Mg O4'
_chemical_name_mineral           Magnesioferrite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.43712
_cell_formula_units_Z            8
_cell_length_b                   8.43712
_cell_length_c                   8.43712
_cell_volume                     600.596
_database_code_amcsd             0003709
_diffrn_ambient_temperature      816.15
_exptl_crystal_density_diffrn    4.424
_exptl_crystal_thermal_history   'cooling T = 543 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Fe2 Mg) O4'
_cod_database_code               9003616
Cation ordering in magnesioferrite, MgFe2O4, to 982 C using in situ synchrotron X-ray powder diffraction Sample: on cooling T = 505 C
Antao, S. M.; Hassan, I.; Parise, J. B.; American Mineralogist 90 (2005) 219–228; doi:10.2138/am.2005.1559

data_9003617
_publ_section_title
;
 Cation ordering in magnesioferrite, MgFe2O4, to 982 C using
 in situ synchrotron X-ray powder diffraction
 Sample: on cooling T = 505 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              219
_journal_page_last               228
_journal_paper_doi               10.2138/am.2005.1559
_journal_volume                  90
_journal_year                    2005
_chemical_formula_sum            'Fe2 Mg O4'
_chemical_name_mineral           Magnesioferrite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.43375
_cell_formula_units_Z            8
_cell_length_b                   8.43375
_cell_length_c                   8.43375
_cell_volume                     599.877
_database_code_amcsd             0003710
_diffrn_ambient_temperature      778.15
_exptl_crystal_density_diffrn    4.429
_exptl_crystal_thermal_history   'cooling T = 505 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Fe2 Mg) O4'
_cod_database_code               9003617
Cation ordering in magnesioferrite, MgFe2O4, to 982 C using in situ synchrotron X-ray powder diffraction Sample: on cooling T = 448 C
Antao, S. M.; Hassan, I.; Parise, J. B.; American Mineralogist 90 (2005) 219–228; doi:10.2138/am.2005.1559

data_9003618
_publ_section_title
;
 Cation ordering in magnesioferrite, MgFe2O4, to 982 C using
 in situ synchrotron X-ray powder diffraction
 Sample: on cooling T = 448 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              219
_journal_page_last               228
_journal_paper_doi               10.2138/am.2005.1559
_journal_volume                  90
_journal_year                    2005
_chemical_formula_sum            'Fe2 Mg O4'
_chemical_name_mineral           Magnesioferrite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.42961
_cell_formula_units_Z            8
_cell_length_b                   8.42961
_cell_length_c                   8.42961
_cell_volume                     598.994
_database_code_amcsd             0003711
_diffrn_ambient_temperature      721.15
_exptl_crystal_density_diffrn    4.435
_exptl_crystal_thermal_history   'cooling T = 448 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Fe2 Mg) O4'
_cod_database_code               9003618
Cation ordering in magnesioferrite, MgFe2O4, to 982 C using in situ synchrotron X-ray powder diffraction Sample: on cooling T = 410 C
Antao, S. M.; Hassan, I.; Parise, J. B.; American Mineralogist 90 (2005) 219–228; doi:10.2138/am.2005.1559

data_9003619
_publ_section_title
;
 Cation ordering in magnesioferrite, MgFe2O4, to 982 C using
 in situ synchrotron X-ray powder diffraction
 Sample: on cooling T = 410 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              219
_journal_page_last               228
_journal_paper_doi               10.2138/am.2005.1559
_journal_volume                  90
_journal_year                    2005
_chemical_formula_sum            'Fe2 Mg O4'
_chemical_name_mineral           Magnesioferrite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.42558
_cell_formula_units_Z            8
_cell_length_b                   8.42558
_cell_length_c                   8.42558
_cell_volume                     598.135
_database_code_amcsd             0003712
_diffrn_ambient_temperature      683.15
_exptl_crystal_density_diffrn    4.442
_exptl_crystal_thermal_history   'cooling T = 410 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Fe2 Mg) O4'
_cod_database_code               9003619
Cation ordering in magnesioferrite, MgFe2O4, to 982 C using in situ synchrotron X-ray powder diffraction Sample: on cooling T = 353 C
Antao, S. M.; Hassan, I.; Parise, J. B.; American Mineralogist 90 (2005) 219–228; doi:10.2138/am.2005.1559

data_9003620
_publ_section_title
;
 Cation ordering in magnesioferrite, MgFe2O4, to 982 C using
 in situ synchrotron X-ray powder diffraction
 Sample: on cooling T = 353 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              219
_journal_page_last               228
_journal_paper_doi               10.2138/am.2005.1559
_journal_volume                  90
_journal_year                    2005
_chemical_formula_sum            'Fe2 Mg O4'
_chemical_name_mineral           Magnesioferrite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.42080
_cell_formula_units_Z            8
_cell_length_b                   8.42080
_cell_length_c                   8.42080
_cell_volume                     597.118
_database_code_amcsd             0003713
_diffrn_ambient_temperature      626.15
_exptl_crystal_density_diffrn    4.449
_exptl_crystal_thermal_history   'cooling T = 353 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Fe2 Mg) O4'
_cod_database_code               9003620
Cation ordering in magnesioferrite, MgFe2O4, to 982 C using in situ synchrotron X-ray powder diffraction Sample: on cooling T = 295 C
Antao, S. M.; Hassan, I.; Parise, J. B.; American Mineralogist 90 (2005) 219–228; doi:10.2138/am.2005.1559

data_9003621
_publ_section_title
;
 Cation ordering in magnesioferrite, MgFe2O4, to 982 C using
 in situ synchrotron X-ray powder diffraction
 Sample: on cooling T = 295 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              219
_journal_page_last               228
_journal_paper_doi               10.2138/am.2005.1559
_journal_volume                  90
_journal_year                    2005
_chemical_formula_sum            'Fe2 Mg O4'
_chemical_name_mineral           Magnesioferrite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.41415
_cell_formula_units_Z            8
_cell_length_b                   8.41415
_cell_length_c                   8.41415
_cell_volume                     595.704
_database_code_amcsd             0003714
_diffrn_ambient_temperature      568.15
_exptl_crystal_density_diffrn    4.460
_exptl_crystal_thermal_history   'cooling T = 295 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Fe2 Mg) O4'
_cod_database_code               9003621
Cation ordering in magnesioferrite, MgFe2O4, to 982 C using in situ synchrotron X-ray powder diffraction Sample: on cooling T = 257 C
Antao, S. M.; Hassan, I.; Parise, J. B.; American Mineralogist 90 (2005) 219–228; doi:10.2138/am.2005.1559

data_9003622
_publ_section_title
;
 Cation ordering in magnesioferrite, MgFe2O4, to 982 C using
 in situ synchrotron X-ray powder diffraction
 Sample: on cooling T = 257 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              219
_journal_page_last               228
_journal_paper_doi               10.2138/am.2005.1559
_journal_volume                  90
_journal_year                    2005
_chemical_formula_sum            'Fe2 Mg O4'
_chemical_name_mineral           Magnesioferrite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.41259
_cell_formula_units_Z            8
_cell_length_b                   8.41259
_cell_length_c                   8.41259
_cell_volume                     595.373
_database_code_amcsd             0003715
_diffrn_ambient_temperature      530.15
_exptl_crystal_density_diffrn    4.462
_exptl_crystal_thermal_history   'cooling T = 257 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Fe2 Mg) O4'
_cod_database_code               9003622
Cation ordering in magnesioferrite, MgFe2O4, to 982 C using in situ synchrotron X-ray powder diffraction Sample: on cooling T = 200 C
Antao, S. M.; Hassan, I.; Parise, J. B.; American Mineralogist 90 (2005) 219–228; doi:10.2138/am.2005.1559

data_9003623
_publ_section_title
;
 Cation ordering in magnesioferrite, MgFe2O4, to 982 C using
 in situ synchrotron X-ray powder diffraction
 Sample: on cooling T = 200 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              219
_journal_page_last               228
_journal_paper_doi               10.2138/am.2005.1559
_journal_volume                  90
_journal_year                    2005
_chemical_formula_sum            'Fe2 Mg O4'
_chemical_name_mineral           Magnesioferrite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.40607
_cell_formula_units_Z            8
_cell_length_b                   8.40607
_cell_length_c                   8.40607
_cell_volume                     593.990
_database_code_amcsd             0003716
_diffrn_ambient_temperature      473.15
_exptl_crystal_density_diffrn    4.473
_exptl_crystal_thermal_history   'cooling T = 200 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Fe2 Mg) O4'
_cod_database_code               9003623
Cation ordering in magnesioferrite, MgFe2O4, to 982 C using in situ synchrotron X-ray powder diffraction Sample: on cooling T = 143 C
Antao, S. M.; Hassan, I.; Parise, J. B.; American Mineralogist 90 (2005) 219–228; doi:10.2138/am.2005.1559

data_9003624
_publ_section_title
;
 Cation ordering in magnesioferrite, MgFe2O4, to 982 C using
 in situ synchrotron X-ray powder diffraction
 Sample: on cooling T = 143 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              219
_journal_page_last               228
_journal_paper_doi               10.2138/am.2005.1559
_journal_volume                  90
_journal_year                    2005
_chemical_formula_sum            'Fe2 Mg O4'
_chemical_name_mineral           Magnesioferrite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.40084
_cell_formula_units_Z            8
_cell_length_b                   8.40084
_cell_length_c                   8.40084
_cell_volume                     592.882
_database_code_amcsd             0003717
_diffrn_ambient_temperature      416.15
_exptl_crystal_density_diffrn    4.481
_exptl_crystal_thermal_history   'cooling T = 143 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Fe2 Mg) O4'
_cod_database_code               9003624
Cation ordering in magnesioferrite, MgFe2O4, to 982 C using in situ synchrotron X-ray powder diffraction Sample: on cooling T = 105 C
Antao, S. M.; Hassan, I.; Parise, J. B.; American Mineralogist 90 (2005) 219–228; doi:10.2138/am.2005.1559

data_9003625
_publ_section_title
;
 Cation ordering in magnesioferrite, MgFe2O4, to 982 C using
 in situ synchrotron X-ray powder diffraction
 Sample: on cooling T = 105 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              219
_journal_page_last               228
_journal_paper_doi               10.2138/am.2005.1559
_journal_volume                  90
_journal_year                    2005
_chemical_formula_sum            'Fe2 Mg O4'
_chemical_name_mineral           Magnesioferrite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.39837
_cell_formula_units_Z            8
_cell_length_b                   8.39837
_cell_length_c                   8.39837
_cell_volume                     592.359
_database_code_amcsd             0003718
_diffrn_ambient_temperature      378.15
_exptl_crystal_density_diffrn    4.485
_exptl_crystal_thermal_history   'cooling T = 105 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Fe2 Mg) O4'
_cod_database_code               9003625
Cation ordering in magnesioferrite, MgFe2O4, to 982 C using in situ synchrotron X-ray powder diffraction Sample: on cooling T = 47 C
Antao, S. M.; Hassan, I.; Parise, J. B.; American Mineralogist 90 (2005) 219–228; doi:10.2138/am.2005.1559

data_9003626
_publ_section_title
;
 Cation ordering in magnesioferrite, MgFe2O4, to 982 C using
 in situ synchrotron X-ray powder diffraction
 Sample: on cooling T = 47 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              219
_journal_page_last               228
_journal_paper_doi               10.2138/am.2005.1559
_journal_volume                  90
_journal_year                    2005
_chemical_formula_sum            'Fe2 Mg O4'
_chemical_name_mineral           Magnesioferrite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.39514
_cell_formula_units_Z            8
_cell_length_b                   8.39514
_cell_length_c                   8.39514
_cell_volume                     591.676
_database_code_amcsd             0003719
_diffrn_ambient_temperature      320.15
_exptl_crystal_density_diffrn    4.490
_exptl_crystal_thermal_history   'cooling T = 47 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Fe2 Mg) O4'
_cod_database_code               9003626